Presentation on theme: "Speaker: C. J. Lee Date: 2009/12/23"— Presentation transcript:
1Speaker: C. J. Lee Date: 2009/12/23 Group meeting: Transparent Conductive Film and Micro/Submicro-Tenile tests by membrane deflection experiment (MDE)Sir, Dr. Du, Dr. Lai, Dr. Chen and everyone good afternoon. Today I will present and report my recent research results.I have two research project. One is transparent conductive film. This project is a cooperative project with Dr. HK Lin of industrial technology research institute.Another is the micro/submicro-tensile tests by membrane deflection experiment, termed MDE.Speaker: C. J. LeeDate: 2009/12/23
2Outline Micro/Submicro-tensile tests Transparent conductive film Mechanical test methods for the thin filmsMembrane deflection experiment(MDE)Preliminary resultsProspectsTransparent conductive filmIntorductionExperimental methodsResultsSummary and SuggestionHere is the outline of this presentation. Firstly, I will present the micro/submicro-tensile tests project. In the part of micro/submicro-tensile tests, I will introduce the mechanical test methods for the thin films and what is the membrane deflection experiment, MDE. Then, report the preliminary results and prospects. That is some improving plane in this project. End the micro/submicro-tensile tests part, I will also introduce the transparent conductive film project, termed TCF project. In the TCF project, firstly, I will introduce what is the transparent conductive film and how to manufacture this transparent conductive film, then report the experimental methods and results. Finally, I will make a brief summary and suggestion for this research project.
3Transparent conductive film What is the Transparent conductive film (TCF)?the films with the exclusive properties of good transparency for visible light and conductivityHow to manufacture this TCF?Generally, a transparent substrate (glass or polymer substrate) being coated some transparent conductive materials, such as Indium tin oxide(ITO), ZnO.Application of TCF:Flat-panel display, solar cells and electromagnetic shielding of CRTs used for video display terminals.
4Transparent conductive film Difficult challenge:TCF coated on flexible substrate could maintain stable conductivity after high cycles bending or high curvature radius bending.Purpose: fabricate a highly flexible TCF with a good reliability on conductivityIf someone TCF are coated on flexible substrate, it will confront a big challenge of maintaining stable conductivity after high cycles bending or high curvature radius.Because the traditional TCF, ITO will appear the crack to influence the conductivity after high cycles bending or high curvature radius. So, in this project, our purpose is fabricate the …..ITO/PET bending@ D < 13 mmNormalized resistance change after repeatedBending as a function of the number of cyclesStandard: normalized resistance change rate < 10%
5Experimental methods TCF structures: Metal layer: Pure Ag Co-sputter Ag-AlCo-sputter Ag-TiCo-sputter Cu-ZrAlloy target: Cu50Zr50Metal layer(Ag, or Amorphous metal, < 10 nm)ITO film (oxide film, ~30 nm)ITO or ZnO film (oxide film, ~30 nm)PET substrate, 125 mmPET substrate, 125 mmMetal layer(Ag, or Amorphous metal, < 10 nm)ITO film (oxide film, ~30 nm)Bi-layer structureTri-layer structureOur design has two different TCF structure, one is the bi-layer structure. In this structure, the metal layer will be coated firstly, then coated the ITO film. Another structure is a sandwich structure. This structure design has been reported in many literatures. Metal layer materials will have ….
6Experimental methods Transmittance and reflectivity measurement: Instrument: N & K analyzerWavelength:Deep ultraviolet-visible-near infrared, nm,1 nm intervalsFilm thickness measurement:Instrument: 3D alpha-step profilometerSheet resistance measurement:Four point probeElement analysis: SEM 6400 EDSCrystalline structure examination:X-ray diffraction, SIEMENS D5000
7Experimental flow chart Alloy design,By adjusting the parameters ofco-sputtering, such as power, metal materials.a-stepEDSXRDBi-layers and Tri-layers depositionN & KFour point probeEvaluation, analysis and modification
8Results Phase diagrams of Ag-Al and Ag-Ti systems Ag-Al system These two figures are Ag-Al and Ag-Ti phase diagram. From these two phase diagram, we know Ag-Al and Ag-Ti are miscible system. However, in alloy design, I hope the alloy element will be Ag as matrix.Ag-Al systemAg-Ti system
9Results Ag-Al system Ag80Al20 Ag71Al29 Ag67Al33 Ag57Al43 Ag47Al53 In Ag-Al co-sputtering, Ag80Al20 will precipitate some small and white particles in gray matrix. However, Ag ratio is lower than 70%, the appearance of co-sputtering films are very clear without precipitation. Very like amorphous film.Ag57Al43Ag47Al53Ag30Al70
10Results Ag-Ti system Ag75Ti25 Ag70Ti30 Ag61Ti39 Ag48Ti52 Ag38Ti62 In Ag-Ti co-sputtering, Ag75Al25 precipitate many gray precipitation in black matrix. White particle may be contamination. However, Ag ratio is lower than 70%, the appearance of co-sputtering films are very clear without precipitation. Very like amorphous film.Ag48Ti52Ag38Ti62
11Results XRD results: The Ag-Al system did not form the fully amorphous except Ag30Al70. The crystallinediffraction peaks of (111) and (200) planesin Ag metal could be observed.The Ag-Ti system did not form the fullyAmorphous. The crystalline diffractionpeaks of (111) and (200) planes in Agmetal could be observed.
12ResultsGrain size estimation based on the peak full width at half maximum (FWHM)Equation: , where the d is grain size, K is Scherrer constant (K=0.94 for the cubic lattices) and l is the wave length of incident Cu Ka radiation (l= nm)AlloyAg71Al29Ag67Al33Ag64Al36Ag57Al43Ag47Al53Size, nm4.05.36.23.62.8Ag75Ti25Ag70Ti30Ag61Ti39Ag48Ti52308.45.14.5
13Results 3 nm metal film coated on Si substrate Ag47Al53 Pure Ag Pure Ag deposition with 3 nm thickness, the morphology is island structure. However, Ag-Al, Ag-Ti and ZrCu are continuous film.Ag48Ti52Zr54Cu46
18Common characteristics Best: First layer is RF gun and lower power,ex: Ag(3 or 6 nm)+ITOSuperior: First layer is the lower power at RF or DCgun and thickerex: ZrCu( 6 nm)+ITOWorse: First layer is the higher power at DC gunex: AgAl( 3 nm)+ITO
19Sputter mechanismAt high powers, the substrate surface, especially of organic substrate, is damaged by the bombardment of the substrate by energetic particles.High power damage of organic substrate surface will induce the discontinuous films to result in the increasing of resistance.Sputter deposition is a method, employing the Ar atom ionization in plasma, therefore,
21Transmittance and electrical properties of Zr50Cu50 film SpecimenTransmitance, % at 550 nmSheet resistance, Ω/□Transmittance, % at 550 nmITO_L8021KITO793.7 K3 nm ZrCu+ITO_L32 K6 nm ZrCu+ITO_L7822 K6 nm ZrCu+ITO761.5 K9 nm ZrCu+ITO_L3.3 K9 nm ZrCu+ITO6312 nm ZrCu+ITO_L5.2 K15 nm ZrCu+ITO_L488 K21 nm ZrCu+ITO_L6026 K
22SummaryThe co-sputtering of Ag-Al and Ag-Ti alloys can not form the fully amorphous of silver matrix.The Ag metallic film showed the good transmittance and conductivity in the TCF of bi-layers and tri-layers structures.The co-sputtering Zr54Cu46 amorphous film exhibited the better transmittance and conductivity than other co-sputtering AgAl and AgTi metallic films in the bi-layers TCF.
23SummaryThe higher power of sputtering should be avoided in order not to damage the surface of organic substrate during coating the first layer film.The Zr50Cu50 amorphous film, using the ZrCu alloy target, could perform the best transmittance in the TCF of bi-layers structure
24Future work and suggestion The Good parameters of sputtering ITO film should be further studied to make the film perform the superior transmittance and conductivity.The co-sputtering Ag-X films should be worthy to research based on pure science perspective.The evaporation or E-beam evaporation might be an appropriate processing route.The cycle bending and small curvature bending will be conducted in ITRI
25AcknowledgementI would like greatly acknowledge the help of S. Y. Sun in wet-etching, lift-off process, nano-indentation, sputtering, resistance measurement, and other miscellaneous things.I would also acknowledge the help of Laiyen in designing the mask pattern, lift-off process, and the help of H.M. Chen in lift-off process and wet-etching.